Functionalized porous Beata A. Zasońska1 silica&maghemite · PDF file 2016. 6....
Embed Size (px)
Transcript of Functionalized porous Beata A. Zasońska1 silica&maghemite · PDF file 2016. 6....
Aim To determine cytotoxicity and effect of silica-coated magnetic nanoparticles (MNPs) on immune response, in particular lymphocyte proliferative activity, phagocytic ac- tivity, and leukocyte respiratory burst and in vitro produc- tion of interleukin-6 (IL-6) and 8 (IL-8), interferon-gamma (IFN-γ), tumor necrosis factor-alpha (TNF-α), and granulo- cyte macrophage colony stimulating factor (GM-CSF).
Methods Maghemite was prepared by coprecipitation of iron salts with ammonia, oxidation with NaOCl and modi- fied by tetramethyl orthosilicate and aminosilanes. Particles were characterized by transmission electron microscopy (TEM), dynamic light scattering (DLS), Fourier-transform in- frared (FTIR), and X-ray photoelectron spectroscopy (XPS). Cytotoxicity and lymphocyte proliferative activity were assessed using [3H]-thymidine incorporation into DNA of proliferating human peripheral blood cells. Phagocytic ac- tivity and leukocyte respiratory burst were measured by flow cytometry; cytokine levels in cell supernatants were determined by ELISA.
Results γ-Fe2O3&SiO2-NH2 MNPs were 13 nm in size. Ac- cording to TEM, they were localized in the cell cytoplasm and extracellular space. Neither cytotoxic effect nor sig- nificant differences in T-lymphocyte and T-dependent B- cell proliferative response were found at particle concen- trations 0.12-75 μg/cm2 after 24, 48, and 72 h incubation. Significantly increased production of IL-6 and 8, and GM- CSF cytokines was observed in the cells treated with 3, 15, and 75 µg of particles/cm2 for 48 h and stimulated with pokeweed mitogen (PHA). No significant changes in TNF-α and IFN-γ production were observed. MNPs did not affect phagocytic activity of monocytes and granulocytes when added to cells for 24 and 48 h. Phagocytic respiratory burst was significantly enhanced in the cultures exposed to 75 µg MNPs/cm2 for 48 h.
Conclusions The cytotoxicity and in vitro immunotoxicity were found to be minimal in the newly developed porous core-shell γ-Fe2O3&SiO2-NH2 magnetic nanoparticles.
Received: January 13, 2016
Accepted: March 24, 2016
Correspondence to: Daniel Horák Department of Polymer Particles Institute of Macromolecular Chemistry Academy of Sciences of the Czech Republic Heyrovského Sq. 2 162 06 Prague 6, Czech Republic firstname.lastname@example.org
Beata A. Zasońska1, Aurélia Líšková2, Miroslava Kuricová2, Jana Tulinská2, Ognen Pop-Georgievski1, Fedor Čiampor3, Ivo Vávra4, Mária Dušinská5, Silvia Ilavská2, Mira Horváthová2, Daniel Horák1
1Institute of Macromolecular Chemistry, Academy of Sciences of the Czech Republic, Prague, Czech Republic
2Medical Faculty, Slovak Medical University, Bratislava, Slovakia
3Institute of Virology, Slovak Academy of Sciences, Bratislava, Slovakia
4Institute of Electrical Engineering, Slovak Academy of Sciences, Bratislava, Slovakia
5Health Effects Laboratory, Department of Environmental Chemistry, NILU-Norwegian Institute for Air Research, Kjeller, Norway
Functionalized porous silica&maghemite core-shell nanoparticles for applications in medicine: design, synthesis, and immunotoxicity
RECOOP for Common Mechanisms of Diseases
Croat Med J. 2016;57:165-78
mailto: email@example.com http://dx.doi.org/10.3325/cmj.2016.57.165
RECOOP for Common Mechanisms of Diseases 166 Croat Med J. 2016;57:165-78
Superparamagnetic nanoparticles containing both non- porous and porous shells have been intensively investigat- ed in recent years with respect to their potential applica- tions in separation of molecules (1), sensors (2), as contrast agents in magnetic resonance imaging (MRI) (3), as well as carriers of drugs and biomolecules (4) for diagnostic (5) and therapeutic purposes (6).
Magnetic nanoparticles (MNPs), such as magnetite (Fe3O4) or maghemite (γ-Fe2O3), received considerable attention for their small size, spherical shape, strong magnetic proper- ties enabling targeting to a specific organ using an external magnetic field (7), and rather low toxicity (8). However, neat (uncoated) iron oxide particles showed toxicity at high dos- es, tendency to aggregate, and high nonspecific adsorption of biomolecules, which is inacceptable for in vitro or in vivo medical applications (9). This can be avoided by surface mod- ifications, such as grafting (coating) and/or encapsulation of MNPs by polymers, which are the most frequently used ma- terials to improve biocompatibility and stability of the iron oxide nanoparticles in aqueous media. Some examples of polymers include dextran, poly(vinyl alcohol) (10), chitosan (11), poly(methyl methacrylate) (12), poly(ethylene glycol) (13), or poly(L-lysine). One of the universal agents to modify the iron oxide surface is also silica (14). This chemically inert inorganic material has a lot of advantages for biomedical ap- plications compared to other materials. It is porous, biocom- patible, modifiable with various functional agents, and has no toxicity at moderate concentrations (15); however silica dust is harmful if inhaled, and induces silicosis. Silica deriva- tives can introduce functional groups, eg, NH2, COOH, SH, on the iron oxide surface to enable immobilization of target biomolecules. Mesoporous silica nanoparticles are thus at- tractive for drug loading and controlled release (16).
The aim of this research was to synthesize γ-Fe2O3, γ-Fe2O3&SiO2, and γ-Fe2O3&SiO2-NH2 MNPs and thorough- ly characterize them. We also aimed to investigate in vitro cytotoxicity and immunotoxicity of the γ-Fe2O3&SiO2-NH2 nanoparticles.
MATerIALS AnD MeTHODS
FeCl2 · 4H2O and FeCl3 · 6H2O were purchased from Flu- ka (Buchs, Switzerland). Sodium hypochlorite solution (5 wt.%) was from Bochemie (Bohumín, Czech Republic). Te- tramethyl orthosilicate (TMOS), (3-aminopropyl)triethox- ysilane (APTES), (3-aminopropyl)dimethylethoxysilane (AP-
DMES), RPMI-1640 medium, phytohemagglutinin (PHA), concanavalin A (Con A), pokeweed mitogen (PWM), L- glutamine, and hydroethidine were purchased from Sig- ma-Aldrich (Steinheim, Germany). Anti-CD3 monoclonal antibody was purchased from Beckman Coulter and fetal calf serum (FCS) from PAA. Fluorescein-labeled Staphylo- coccus aureus bacteria and opsonizing reagent were pur- chased from Molecular Probes (Eugene, OR, USA). Cationic surfactant, cetyltrimethylammonium bromide (CTAB) was purchased from Lachema (Brno, Czech Republic). Am- monium hydroxide solution (25%) and ethanol were pur- chased from Lach-Ner (Neratovice, Czech Republic). Gen- tamycin was purchased from Sandoz (Bratislava, Slovakia), cyclophosphamide (Cyf ) from Baxter (Deerfield, IL, USA), and [3H]-thymidine from Moravek Biochemicals (Brea, CA, USA). Scintillation fluid was purchased from Perkin Elmer (Waltham, MA, USA). Ultrapure Q-water ultrafiltered on a Milli-Q Gradient A10 system (Millipore, Molsheim, France) was used for preparation of the solutions. ELISA sets were purchased from Affymetrix e-Biosciences.
Preparation of γ-Fe2O3 nanoparticles
Iron oxide nanoparticles were prepared from iron(III) chlo- ride and iron(II) chloride by a standard procedure (17). Aqueous 0.2 M FeCl3 (100 mL), 0.2 M FeCl2 (50 mL), and 0.5 M NH4OH (100 mL) solutions were sonicated (Sonicator W-385; Heat Systems-Ultrasonics; Farmingdale, USA) for 5 min. The mixture was added to 3.3 wt.% NH4OH (460 mL) and stirred at 23°C for 1 h (200 rpm). Magnetite was mag- netically separated and washed by Q-water until peptiza- tion. Then, 5 wt.% sodium hypochlorite solution (16 mL) was added and the system sonicated for 5 min. The precip- itate was magnetically separated and repeatedly washed with Q-water until formation of γ-Fe2O3 colloid.
Synthesis of porous core-shell γ-Fe2O3&SiO2-nH2 nanoparticles
First, silica shell was introduced on the particles by modi- fication of Stöber method using hydrolysis and condensa- tion of TMOS (18). In a typical experiment, ethanol (60 mL), water (3 mL), and 25 wt.% ammonia (0.3 mL) were mixed with γ-Fe2O3 (150 mg) for 5 min. TMOS (0.1 mL) was added and the mixture stirred (400 rpm) at 50°C for 16 h. The re- sulting γ-Fe2O3&SiO2 colloid was three times washed with ethanol using magnetic separation.
The second (porous) shell containing amino groups on the surface was introduced by modification of γ-Fe2O3&SiO2
167Zasońska et al: Functionalized silica&maghemite core-shell nanoparticles
nanoparticles with APTES/APDMES mixture (Figure 1). Briefly, γ-Fe2O3&SiO2 nanoparticles were dispersed in etha- nol (60 mL) and CTAB (0.15 g), APTES (0.05 mL), APDMES (0.05 mL), and water (1 mL) were added. The mixture was stirred using an anchor-type stirrer (400 rpm) at 50°C for 24 h. After completion of the reaction, the resulting porous γ-Fe2O3&SiO2-NH2 particles were washed using magnetic separation (5 times with ethanol and 3 times with water) and centrifugation (3 times).
Characterization of nanoparticles
The synthesized nanoparticles were characterized by a Tecnai Spirit G2 transmission electron microscope (TEM; FEI) and number- (Dn) and weight-average particle diam- eter (Dw) and polydispersity index (PDI = Dw/Dn) were cal- culated by analyzing ca. 400 particles. The hydrodynamic particle size (Dh) of γ-Fe2O3 and γ-Fe2O3&SiO2 and polydis- persity PI (0-1) was determined by dynamic light scat- tering (DLS) using a Zetasizer Nano-ZS Model ZEN3600 instrument (Malvern Instruments; Malvern, UK). Fourier- transform infrared (FTIR) spect